Thermo- and light-triggered reversible interconversion of dysprosium-anthracene complexes and their responsive optical, magnetic and dielectric properties.
Huang, Xin-Da; Wen, Ge-Hua; Bao, Song-Song; Jia, Jia-Ge; Zheng, Li-Min; Chemical science 12 (2020) 929–937; doi:10.1039/d0sc04851h

data_1559656
_publ_section_title
;
 Thermo- and light-triggered reversible interconversion of
 dysprosium-anthracene complexes and their responsive optical, magnetic
 and dielectric properties.
;
_journal_issue                   3
_journal_name_full               'Chemical science'
_journal_page_first              929
_journal_page_last               937
_journal_paper_doi               10.1039/d0sc04851h
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety         'C51 H52 Dy N5 O8 P2 S3'
_chemical_formula_sum            'C51 H52 Dy N5 O8 P2 S3'
_chemical_formula_weight         1183.59
_chemical_name_systematic        1RT
_chemical_properties_physical    Photo-sensitive
_space_group_crystal_system      monoclinic
_space_group_IT_number           11
_space_group_name_Hall           '-P 2yb'
_space_group_name_H-M_alt        'P 1 21/m 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2020-07-19 deposited with the CCDC.	2020-11-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 107.460(10)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.081(4)
_cell_length_b                   24.946(8)
_cell_length_c                   11.246(4)
_cell_measurement_reflns_used    9446
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      27.058
_cell_measurement_theta_min      2.2725
_cell_volume                     2697.8(17)
_computing_cell_refinement       'Bruker APEX3'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker APEX3'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2014/5 (Sheldrick, 2014)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker D8 Venture'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0430
_diffrn_reflns_av_unetI/netI     0.0382
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.991
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       31
_diffrn_reflns_limit_k_min       -31
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            24432
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.991
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.136
_diffrn_reflns_theta_min         2.270
_exptl_absorpt_coefficient_mu    1.616
_exptl_absorpt_correction_T_max  0.882
_exptl_absorpt_correction_T_min  0.679
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS 2016/2'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.457
_exptl_crystal_description       block
_exptl_crystal_F_000             1202
_exptl_crystal_preparation       'Magnetic properties,Luminescent,Dielectric'
_exptl_crystal_recrystallization_method 'Vapour deposition'
_exptl_crystal_size_max          0.240
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.080
_refine_diff_density_max         0.856
_refine_diff_density_min         -0.642
_refine_diff_density_rms         0.073
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.048
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     422
_refine_ls_number_reflns         6050
_refine_ls_number_restraints     382
_refine_ls_restrained_S_all      1.067
_refine_ls_R_factor_all          0.0592
_refine_ls_R_factor_gt           0.0456
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0564P)^2^+2.3307P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1112
_refine_ls_wR_factor_ref         0.1201
_reflns_Friedel_coverage         0.000
_reflns_number_gt                5000
_reflns_number_total             6050
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0sc04851h2.cif
_cod_data_source_block           1RT
_cod_depositor_comments
;Adding full bibliography for 1559656--1559657.cif.

 Adding full bibliography for 1559656--1559657.cif.
;
_cod_original_cell_volume        2697.7(15)
_cod_original_sg_symbol_H-M      'P 21/m'
_cod_database_code               1559656
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.698
_shelx_estimated_absorpt_t_max   0.882
_shelx_res_checksum              99100